Solution Manual for Materials Science and Engineering An Introduction 9th Edition by William D. Callister and David G. Rethwisch
Link download full: https://digitalcontentmarket.org/download/solutionmanualformaterialsscienceandengineeringanintroduction9theditionbycallisterandrethwisch/
CHAPTER 4
IMPERFECTIONS IN SOLIDS
PROBLEM SOLUTIONS
Vacancies and SelfInterstitials 4.1 The equilibrium fraction of lattice sites that are vacant in silver (Ag) at 700 C is 2 106. Calculate the number of vacancies (per meter cubed) at 700C. Assume a density of 10.35 g/cm3 for Ag. Solution This problem is solved using two steps: (1) calculate the total number of lattice sites in silver, NAg, using Equation 4.2; and (2) multiply this number by fraction of lattice that are vacant, 2 106. The parameter NAg is related to the density, (), Avogadro's number (NA), and the atomic weight (AAg=107.87 g/mol, from inside the front cover) according to Equation 4.2 as
N Ag =
=
N A rAg AAg
(6.022 ´ 1023 atoms/mol)(10.35 g/cm3 )(106 cm3 /m3 ) 107.87 g/mol = 5.78 1028 atoms/m3
The number of vacancies per meter cubed in silver at 700C, Nv, is determined as follows:
Nv = (2 ´10 6 )N Ag
= (2 ´ 106 )(5.78 ´ 1028 atoms/m3 ) = 1.156 ´ 1023 vacancies/m3
4.2 For some hypothetical metal, the equilibrium number of vacancies at 900 C is 2.3 1025 m3. If the density and atomic weight of this metal are 7.40 g/cm3 and 85.5 g/mol, respectively, calculate the fraction of vacancies for this metal at 900C. Solution This problem is solved using two steps: (1) calculate the total number of lattice sites in silver, N, using Equation 4.2, and (2) take the ratio of the equilibrium number of vacancies given in the problem statement (Nv = 2.3 1025 m3) and this value of N. From Equation 4.2
N=
=
NAr A
(6.022 ´ 10 23 atoms/mol)(7.40 g/cm3 )(106 cm3 /m3 ) 85.5 g/mol
= 5.21 ´1028 atoms/m3 The fraction of vacancies is equal to the Nv/N ratio, which is computed as follows:
Nv 2.3 ´ 1025 m 3 = N 5.21 ´ 1028 atoms/m3
= 4.41 ´ 10 4
4.3 (a) Calculate the fraction of atom sites that are vacant for copper (Cu) at its melting temperature of 1084°C (1357 K). Assume an energy for vacancy formation of 0.90 eV/atom. (b) Repeat this calculation at room temperature (298 K). (c) What is ratio of Nv /N(1357 K) and Nv /N(298 K)? Solution (a) In order to compute the fraction of atom sites that are vacant in copper at 1357 K, we must employ Equation 4.1. As stated in the problem, Qv = 0.90 eV/atom. Thus,
Nv = exp N
é ù æ Qv ö 0.90 eV/atom ú ç  kT ÷ = exp ê 5 è ø êë (8.62 ´ 10 eV/atomK ) (1357 K) úû
= 4.56 ´ 104 = N v /N (1357 K) (b) We repeat this computation at room temperature (298 K), as follows:
Nv = exp N
é ù æ Qv ö 0.90 eV/atom ú ç  kT ÷ = exp ê è ø êë (8.62 ´ 105 eV/atomK ) (298 K) úû
= 6.08 ´ 1016 = N v /N (298 K) (c) And, finally the ratio of Nv /N(1357 K) and Nv /N(298 K) is equal to the following:
N v /N(1357 K) 4.56 ´ 10 4 = = 7.5 ´ 1011 N v /N(298 K) 6.08 ´ 10 16
4.4 Calculate the number of vacancies per cubic meter in gold (Au) at 900°C. The energy for vacancy formation is 0.98 eV/atom. Furthermore, the density and atomic weight for Au are 18.63 g/cm 3 (at 900°C) and 196.9 g/mol, respectively. Solution Determination of the number of vacancies per cubic meter in gold at 900C (1173 K) requires the utilization of Equations 4.1 and 4.2 as follows:
æ Q ö N r æ Q ö N v = N exp ç  v ÷ = A Au exp ç  v ÷ AAu è kT ø è kT ø Inserting into this expression he density and atomic weight values for gold leads to the following:
Nv =
é ù (6.022 ´ 1023 atoms/mol)(18.63 g/cm3 ) 0.98 eV/atom exp ê ú 5 196.9 g/mol êë (8.62 ´ 10 eV/atomK)(1173 K) úû
= 3.52 ´ 1018 cm3 = 3.52 ´ 1024 m3
4.5 Calculate the energy for vacancy formation in nickel (Ni), given that the equilibrium number of vacancies at 850°C (1123 K) is 4.7 × 10 22 m–3. The atomic weight and density (at 850°C) for Ni are, respectively, 58.69 g/mol and 8.80 g/cm3.
Solution This problem calls for the computation of the activation energy for vacancy formation in nickel. Upon examination of Equation 4.1, all parameters besides Qv are given except N, the total number of atomic sites. However, N is related to the density, (), Avogadro's number (NA), and the atomic weight (A) according to Equation 4.2 as
N =
=
N A r Ni ANi
(6.022 ´ 1023 atoms/mol)(8.80 g/cm3 ) 58.69 g/mol
= 9.03 1022 atoms/cm3 = 9.03 1028 atoms/m3 Now, taking natural logarithms of both sides of Equation 4.1, yields he following
ln N v = ln N 
Qv kT
We make Qv the dependent variable after some algebraic manipulation as
æN ö Qv =  kT ln ç v ÷ è Nø Incorporation into this expression, values for Nv (determined above as 9.03 1028 atoms/m3), N (provided in the problem statement, 4.7 × 1022 m–3 ). T (850C = 1123 K) and k, leads to the following:
é 4.7 ´ 1022 m 3 ù Qv =  (8.62 ´ 105 eV/atomK) (1123 K) ln ê 28 3 ú êë 9.03 ´ 10 m úû = 1.40 eV/atom
Impurities in Solids 4.6 Atomic radius, crystal structure, electronegativity, and the most common valence are given in the following table for several elements; for those that are nonmetals, only atomic radii are indicated. Element
Atomic Radius (nm)
Crystal Structure
Electronegativity
Valence
Ni C H O Ag Al Co Cr Fe Pt Zn
0.1246 0.071 0.046 0.060 0.1445 0.1431 0.1253 0.1249 0.1241 0.1387 0.1332
FCC
1.8
+2
FCC FCC HCP BCC BCC FCC HCP
1.4 1.5 1.7 1.6 1.7 1.5 1.7
+1 +3 +2 +3 +2 +2 +2
Which of these elements would you expect to form the following with nickel: (a) A substitutional solid solution having complete solubility (b) A substitutional solid solution of incomplete solubility (c) An interstitial solid solution
Solution For complete substitutional solubility the four HumeRothery rules must be satisfied: (1) the difference in atomic radii between Ni and the other element (R%) must be less than ±15%; (2) the crystal structures must be the same; (3) the electronegativities must be similar; and (4) the valences should be the same.
Element
R%
Ni C H O Ag Al Co Cr Fe Pt Zn
–43 –63 –52 +16 +15 +0.6 +0.2 0.4 +11 +7
Crystal Structure
Electronegativity
FCC
FCC FCC HCP BCC BCC FCC HCP
Valence 2+
0.4 0.3 0.1 0.2 0.1 0.3 0.1
1+ 3+ 2+ 3+ 2+ 2+ 2+
(a) Pt is the only element that meets all of the criteria and thus forms a substitutional solid solution having complete solubility. At elevated temperatures Co and Fe experience allotropic transformations to the FCC crystal structure, and thus display complete solid solubility at these temperatures. (b) Ag, Al, Co, Cr, Fe, and Zn form substitutional solid solutions of incomplete solubility. All these metals have either BCC or HCP crystal structures, and/or the difference between their atomic radii and that for Ni are greater than Âą15%, and/or have a valence different than 2+. (c) C, H, and O form interstitial solid solutions. These elements have atomic radii that are significantly smaller than the atomic radius of Ni.
4.7 Which of the following systems (i.e., pair of metals) would you expect to exhibit complete solid solubility? Explain your answers. (a) CrV (b) MgZn (c) AlZr (d) AgAu (e) PbPt
Solution In order for there to be complete solubility (substitutional) for each pair of metals, the four HumeRothery rules must be satisfied: (1) the difference in atomic radii between Ni and the other element (ď „R%) must be less than Âą15%; (2) the crystal structures must be the same; (3) the electronegativities must be similar; and (4) the valences should be the same.
(a) A comparison of these four criteria for the CrV system is given below: Metal
Atomic Radius (nm)
Crystal Structure
Electronegativity
Valence
Cr
0.125
BCC
1.6
+3
V
0.132
BCC
1.5
+5 (+3)
For chromium and vanadium, the percent difference in atomic radii is approximately 6%, the crystal structures are the same (BCC), and there is very little difference in their electronegativities. The most common valence for Cr is +3; although the most common valence of V is +5, it can also exist as +3. Therefore, chromium and vanadium are completely soluble in one another.
(b) A comparison of these four criteria for the MgZn system is given below: Metal
Atomic Radius (nm)
Crystal Structure
Electronegativity
Valence
Mg
0.160
HCP
1.3
+2
Zn
0.133
HCP
1.7
+2
For magnesium and zinc, the percent difference in atomic radii is approximately 17%, the crystal structures are the same (HCP), and there is some difference in their electronegativities (1.3 vs. 1.7). The most common valence for both Mg and Zn is +2. Magnesium and zinc are not completely soluble in one another, primarily because of the difference in atomic radii.
(c) A comparison of these four criteria for the AlZr system is given below:
Metal
Atomic Radius (nm)
Crystal Structure
Electronegativity
Valence
Al
0.143
FCC
1.5
+3
Zr
0.159
HCP
1.2
+4
For aluminum and zirconium, the percent difference in atomic radii is approximately 11%, the crystal structures are different (FCC and HCP), there is some difference in their electronegativities (1.5 vs. 1.2). The most common valences for Al and Zr are +3 and +4, respectively. Aluminum and zirconium are not completely soluble in one another, primarily because of the difference in crystal structures.
(d) A comparison of these four criteria for the AgAu system is given below:
Metal
Atomic Radius (nm)
Crystal Structure
Electronegativity
Valence
Ag
0.144
FCC
1.4
+1
Au
0.144
FCC
1.4
+1
For silver and gold, the atomic radii are the same, the crystal structures are the same (FCC), their electronegativities are the same (1.4), and their common valences are +1. Silver and gold are completely soluble in one another because all four criteria are satisfied.
(d) A comparison of these four criteria for the PbPt system is given below: Metal
Atomic Radius (nm)
Crystal Structure
Electronegativity
Valence
Pb
0.175
FCC
1.6
+2
Pt
0.139
FCC
1.5
+2
For lead and platinum, the percent difference in atomic radii is approximately 20%, the crystal structures are the same (FCC), their electronegativities are nearly the same (1.6 vs. 1.5), and the most common valence for both of them is +2. Lead and platinum are not completely soluble in one another, primarily because of the difference in atomic radii.
4.8 (a) Compute the radius r of an impurity atom that will just fit into an FCC octahedral site in terms of the atomic radius R of the host atom (without introducing lattice strains). (b) Repeat part (a) for the FCC tetrahedral site. (Note: You may want to consult Figure 4.3a.)
Solution (a) In the drawing below is shown the atoms on the (100) face of an FCC unit cell; the small circle represents an impurity atom that just fits within the octahedral interstitial site that is located at the center of the unit cell edge.
The diameter of an atom that will just fit into this site (2r) is just the difference between that unit cell edge length (a) and the radii of the two host atoms that are located on either side of the site (R); that is 2r = a â€“ 2R However, for FCC a is related to R according to Equation 3.1 as a = 2R 2 ; therefore, solving for r from the above equation gives
r=
a  2R 2R 2  2R = = 0.414R 2 2
(b) Drawing (a) below shows one quadrant of an FCC unit cell, which is a cube; corners of the tetrahedron correspond to atoms that are labeled A, B, C, and D. These corresponding atom positions are noted in the FCC unit cell in drawing (b). In both of these drawings, atoms have been reduced from their normal sizes for clarity. The interstitial atom resides at the center of the tetrahedron, which is designated as point E, in both (a) and (b).
Let us now express the host and interstitial atom radii in terms of the cube edge length, designated as a. From Figure (a), the spheres located at positions A and B touch each other along the bottom face diagonal. Thus,
AB = 2 R But
(AB)2 = a2 + a2 = 2a2 or
AB = a 2 = 2 R And
a=
2R 2
There will also be an anion located at the corner, point F (not drawn), and the cube diagonal AEF will be related to the atomic radii as
AEF = 2 (r + R)
(The line AEF has not been drawn to avoid confusion.) From the triangle ABF
(AB)2 + (FB)2 = (AEF)2
(P4.8a)
But,
FB = a =
2R 2
and
AB = 2 R from above. Substitution of the parameters involving r and R noted above into Equation P4.8a leads to the following: 2
(2 R)2 + æç ö÷ = éë2 (r + R)ùû è 2ø 2R
Solving for r leads to
æ 6  2ö r = Rç ÷ = 0.225R 2 è ø
2
4.9 Compute the radius r of an impurity atom that will just fit into a BCC tetrahedral site in terms of the atomic radius R of the host atom (without introducing lattice strains). (Note: You may want to consult Figure 4.3b.)
Solution A (100) face of a BCC unit cell is shown below.
The interstitial atom that just fits into this interstitial site is shown by the small circle. It is situated in the plane of this (100) face, midway between the two vertical unit cell edges, and one quarter of the distance between the bottom and top cell edges. From the right triangle` defined by the three arrows we may write 2
2
æ aö æ aö 2 çè 2 ÷ø + çè 4 ÷ø = (R + r ) However, from Equation 3.4, a =
4R
, and, therefore, making this substitution, the above equation takes the form
3 2
2
æ 4R ö æ 4R ö 2 2 çè ÷ø + çè ÷ = R + 2R r + r 2 3 4 3ø After rearrangement the following quadratic equation results in:
r 2 + 2Rr  0.667R 2 = 0 And upon solving for r:
r=
(2R) Âą (2R)2  (4)(1)(0.667R2 ) 2
=
2R Âą 2.582R 2
And, finally
2R + 2.582R = 0.291R 2 2R  2.582R r() = =  2.291R 2 r(+) =
Of course, only the r(+) root is possible, and, therefore, r = 0.291R.
4.10 (a) Using the result of Problem 4.8(a), compute the radius of an octahedral interstitial site in FCC iron. (b) On the basis of this result and the answer to Problem 4.9, explain why a higher concentration of carbon will dissolve in FCC iron than in iron that has a BCC crystal structure.
Solution (a) From Problem 4.8(a), the radius of an octahedral interstitial site, r, is related to the atomic radius of the host material according to r = 0.414R. The atomic radius of an iron atom is 0.124 nm; therefore, the radius of this octahedral site in iron is
rFe(Oct) = 0.414RFe = (0.414)(0.124 nm) = 0.051 nm (b) Carbon atoms are situated in octahedral sites in FCC iron, and, for BCC iron, in tetrahedral sites. The relationship between r and R for BCC iron, as determined in problem 4.9 is r = 0.291R. Therefore, in BCC iron, the radius of the tetrahedral site is
rFe(Tet) = 0.291RFe = (0.291)(0.124 nm) = 0.036 nm Because the radius of the octahedral site in FCC iron (0.051 nm) is greater the radius of the tetrahedral site in BCC iron (0.036 nm), a higher concentration of carbon will dissolve in FCC.
4.11 (a) For BCC iron, compute the radius of a tetrahedral interstitial site. (See the result of Problem 4.9.) (b)
Lattice strains are imposed on iron atoms surrounding this site when carbon atoms occupy it.
Compute the approximate magnitude of this strain by taking the difference between the carbon atom radius and the site radius and then dividing this difference by the site radius.
Solution (a) The relationship between r and R for BCC iron, as determined in problem 4.9 is r = 0.291R. Therefore, in BCC iron, the radius of the tetrahedral site is
rFe(Tet) = 0.291RFe = (0.291)(0.124 nm) = 0.036 nm (b) The radius of a carbon atom (rC) is 0.071 nm (as taken from the inside cover of the book). The lattice strain introduced by a carbon atom the is situated on a BCC tetrahedral site is determined as follows:
Lattice strain =
rC  rFe(Tet) rFe(Tet)
=
0.071 nm  0.036 nm = 0.97 0.036 nm
Specification of Composition 4.12 Derive the following equations: (a) Equation 4.7a (b) Equation 4.9a (c) Equation 4.10a (d) Equation 4.11b
Solution (a) This problem asks that we derive Equation 4.7a. To begin, C1 is defined according to Equation 4.3a as
C1 =
m1 ´ 100 m1 + m2
or, equivalently
C1 =
m1¢ m1¢ + m2¢
´ 100
where the primed m's indicate masses in grams. From Equation 4.4 we may write
m1¢ = nm1 A1 m2¢ = nm2 A2 And, substitution into the C1 expression above
C1 =
nm1 A1 ´ 100 nm1 A1 + nm2 A2
From Equation 4.5a it is the case that
nm1 =
C1¢ ( nm1 + nm2 ) 100
nm2 =
C2¢ ( nm1 + nm2 ) 100
And substitution of these expressions into the above equation (for C1) leads to
C1 =
C1¢ A1 C1¢ A1 + C2¢ A2
´ 100
which is just Equation 4.7a. (b) This part of the problem asks that we derive Equation 4.9a. To begin, C1¢¢ is defined as the mass of component 1 per unit volume of alloy, or
m1 V
C1¢¢ =
If we assume that the total alloy volume V is equal to the sum of the volumes of the two constituentsi.e., V = V1 + V2—then
C1¢¢ =
m1 V1 + V2
Furthermore, the volume of each constituent is related to its density and mass as
V1 =
V2 =
m1
r1
m2
r2
This leads to
C1¢¢ =
m1 m1
r1
+
m2
r2
From Equation 4.3a, m and m may be expressed as follows: 1
2
m1 =
C1 ( m1 + m2 ) 100
m2 =
C2 ( m1 + m2 ) 100
Substitution of these equations into the preceding expression (for C1¢¢ ) yields
C1 ( m1 + m2 ) 100 C1¢¢ = C1 ( m1 + m2 ) C2 ( m1 + m2 ) 100 100 +
r1 =
r2
C1 C1 C2 +
r1
r2
If the densities 1 and 2 are given in units of g/cm3, then conversion to units of kg/m3 requires that we multiply this equation by 103, inasmuch as 1 g/cm3 = 103 kg/m3 Therefore, the previous equation takes the form
C1¢¢ =
C1
r1
C1 ´ 103 C2 +
r2
the desired expression. (c) Now we are asked to derive Equation 4.10a. The density of an alloy ave is just the total alloy mass M divided by its volume V
rave =
M V
Or, in terms of the component elements 1 and 2
rave =
m1 + m2 V1 + V2
[Note: Here it is assumed that the total alloy volume is equal to the separate volumes of the individual components, which is only an approximation; normally V will not be exactly equal to (V1 + V2)]. Each of V1 and V2 may be expressed in terms of its mass and density as,
V1 =
m1
r1
V2 =
m2
r2
When these expressions are substituted into the above equation (for ave), we get
rave =
m1 + m2 m1 m2 +
r1
r2
Furthermore, from Equation 4.3a
m1 =
C1 ( m1 + m2 ) 100
m2 =
C2 ( m1 + m2 ) 100
Which, when substituted into the above expression yields ave
rave =
m1 + m2 C1 ( m1 + m2 ) C2 ( m1 + m2 ) 100 100 +
r1
r2
And, finally, this equation reduces to
rave =
100 C1 C2 +
r1
r2
(d) And, finally, the derivation of Equation 4.11b for Aave is requested. The alloy average molecular weight is just the ratio of total alloy mass in grams M ¢ and the total number of moles in the alloy Nm. That is
Aave =
m¢ + m2¢ M' = 1 N m nm1 + nm2
But using Equation 4.4 we may write
m1¢ = nm1 A1
m2¢ = nm2 A2 Which, when substituted into the above Aave expression yields
Aave =
n A +n A M¢ = m1 1 m2 2 Nm nm1 + nm2
Furthermore, from Equation 4.5a
nm1 =
C1¢ ( nm1 + nm2 ) 100
nm2 =
C2¢ ( nm1 + nm2 ) 100
Thus, substitution of these expressions into the above equation for Aave yields
Aave
C1¢ A1 (nm1 + nm2 ) C2¢ A2 (nm1 + nm2 ) + 100 100 = nm1 + nm2
=
which is the desired result.
C1¢ A1 + C2¢ A2 100
4.13 What is the composition, in atom percent, of an alloy that consists of 92.5 wt% Ag and 7.5 wt% Cu?
Solution In order to compute composition, in atom percent, of a 92.5 wt% Ag7.5 wt% Cu alloy, we employ Equation 4.6 given the atomic weights of silver and copper (found on the inside of the book's cover): AAg = 107.87 g/mol ACu = 63.55 g/mol These compositions in atom percent are determined as follows:
¢= CAg
=
CAg ACu CAg ACu + CCu AAg
´ 100
(92.5)(63.55 g/mol) ´ 100 (92.5)(63.55 g/mol) + (7.5)(107.87g/mol)
= 87.9 at%
¢= CCu
=
CCu AAg CAg ACu + CCu AAg
´ 100
(7.5)(107.87 g / mol) ´ 100 (92.5)(63.55 g / mol) + (7.5)(107.87g / mol)
= 12.1 at%
4.14 What is the composition, in atom percent, of an alloy that consists of 5.5 wt% Pb and 94.5 wt% Sn?
Solution In order to compute composition, in atom percent, of a 5.5 wt% Pb94.5 wt% Sn alloy, we employ Equation 4.6 given the atomic weights of lead and tin (found on the inside of the book's cover): APb = 207.2 g/mol ASn = 118.71 g/mol These compositions in atom percent are determined as follows:
¢= CPb
=
CPb ASn
CPb ASn + CSn APb
´ 100
(5.5)(118.71 g/mol) ´ 100 (5.5)(118.71 g/mol) + (94.5)(207.2 g/mol)
= 3.23 at%
¢= CSn
=
CSn APb
CPb ASn + CSn APb
´ 100
(94.5)(207.2 g/mol) ´ 100 (5.5)(118.71 g/mol) + (94.5)(207.2 g/mol)
= 96.77 at%
4.15 What is the composition, in weight percent, of an alloy that consists of 5 at% Cu and 95 at% Pt?
Solution In order to compute composition, in weight percent, of a 5 at% Cu95 at% Pt alloy, we employ Equation 4.7 given the atomic weights of copper and platinum (found on the inside of the book's cover): ACu = 63.55 g/mol APt = 195.08 g/mol These compositions in weight percent are determined as follows:
CCu =
=
CCu ¢ ACu ´ 100 CCu ¢ ACu + CPt ¢ APt
(5)(63.55 g/mol) ´ 100 (5)(63.55 g/mol) + (95)(195.08 g/mol) = 1.68 wt%
CPt =
=
CPt ¢ APt ´ 100 CCu ¢ ACu + CPt ¢ APt
(95)(195.08 g/mol) ´ 100 (5)(63.55 g/mol) + (95)(195.08 g/mol) = 98.32 wt%
4.16 Calculate the composition, in weight percent, of an alloy that contains 105 kg of iron, 0.2 kg of carbon, and 1.0 kg of chromium.
Solution The concentration, in weight percent, of an element in an alloy may be computed using Equation 4.3b. For this alloy, the concentration of iron (CFe) is just
CFe =
=
mFe ´ 100 mFe + mC + mCr
105 kg ´ 100 = 98.87 wt% 105 kg + 0.2 kg + 1.0 kg
Similarly, for carbon
CC =
0.2 kg ´ 100 = 0.19 wt% 105 kg + 0.2 kg + 1.0 kg
CCr =
1.0 kg ´ 100 = 0.94 wt% 105 kg + 0.2 kg + 1.0 kg
And for chromium
4.17 What is the composition, in atom percent, of an alloy that contains 33 g of copper and 47 g of zinc?
Solution The concentration of an element in an alloy, in atom percent, may be computed using Equation 4.5a. However, it first becomes necessary to compute the number of moles of both Cu and Zn, using Equation 4.4. Atomic weights of copper and zinc (found on the inside of the book's cover) are as follows: ACu = 63.55 g/mol AZn = 65.41 g/mol
Thus, the number of moles of Cu is just
nm
=
Cu
m¢ Cu
ACu
=
33 g = 0.519 mol 63.55 g/mol
Likewise, for Zn
nm
=
Zn
47 g = 0.719 mol 65.41 g/mol
Now, use of Equation 4.5a yields
CCu ¢ =
nm
Cu
nm
Cu
=
+ nm
´ 100
Zn
0.519 mol ´ 100 = 41.9 at% 0.519 mol + 0.719 mol
Also,
CZn ¢ =
0.719 mol ´ 100 = 58.1 at% 0.519 mol + 0.719 mol
4.18 What is the composition, in atom percent, of an alloy that contains 44.5 lb m of Ag, 83.7 lbm of Au, and 5.3 lbm of Cu? Solution In this problem we are asked to determine the concentrations, in atom percent, of the AgAuCu alloy. It is first necessary to convert the amounts of Ag, Au, and Cu into grams.
mAg ¢ = (44.5 lbm )(453.6 g/lbm ) = 20,185 g
mAu ¢ = (83.7 lbm )(453.6 g/lbm ) = 37,966 g
mCu ¢ = (5.3 lbm )(453.6 g/lbm ) = 2,404 g These masses must next be converted into moles (Equation 4.4), as
nm
mAg ¢
=
AAg
Ag
nm
=
Au
nm
Cu
=
20,185 g = 187.1 mol 107.87 g/mol
37,966 g = 192.8 mol 196.97 g/mol
=
2,404 g = 37.8 mol 63.55 g/mol
Now, employment of Equation 4.5b, gives
CAg ¢ =
nm
Ag
nm + nm Ag
=
Au
+ nm
´ 100
Cu
187.1 mol ´ 100 = 44.8 at% 187.1 mol + 192.8 mol + 37.8 mol
CAu ¢ =
192.8 mol ´ 100 = 46.2 at% 187.1 mol + 192.8 mol + 37.8 mol
CCu ¢ =
37.8 mol ´ 100 = 9.0 at% 187.1 mol + 192.8 mol + 37.8 mol
4.19 Convert the atom percent composition in Problem 4.18 to weight percent.
Solution This problem calls for a conversion of composition in atom percent to composition in weight percent. The composition in atom percent for Problem 4.18 is 44.8 at% Ag, 46.2 at% Au, and 9.0 at% Cu. Modification of Equation 4.7 to take into account a threecomponent alloy leads to the following
CAg =
=
CAg ¢ AAg CAg ¢ AAg + CAu ¢ AAu + CCu ¢ ACu
´ 100
(44.8)(107.87 g/mol) ´ 100 (44.8)(107.87 g/mol) + (46.2)(196.97 g/mol) + (9.0)(63.55 g/mol) = 33.3 wt%
CAu =
=
CAu ¢ AAu ´ 100 CAg ¢ AAg + CAu ¢ AAu + CCu ¢ ACu
(46.2)(196.97 g/mol) ´ 100 (44.8)(107.87 g/mol) + (46.2)(196.97 g/mol) + (9.0)(63.55 g/mol) = 62.7 wt%
CCu =
=
CCu ¢ ACu ´ 100 CAg ¢ AAg + CAu ¢ AAu + CCu ¢ ACu
(9.0)(63.55 g/mol) ´ 100 (44.8)(107.87 g/mol) + (46.2)(196.97 g/mol) + (9.0)(63.55 g/mol)
= 4.0 wt%
4.20 Calculate the number of atoms per cubic meter in Pb.
Solution This problem calls for a determination of the number of atoms per cubic meter for lead. In order to solve this problem, one must employ Equation 4.2,
N=
N A r Pb APb
The density of Pb (from the table inside of the front cover) is 11.35 g/cm3, while its atomic weight is 207.2 g/mol. Thus,
N=
(6.022 ´ 1023 atoms/mol)(11.35 g/cm3) 207.2 g/mol
= 3.30 ´ 1022 atoms/cm3 = 3.30 ´ 1028 atoms/m3
4.21 Calculate the number of atoms per cubic meter in Cr.
Solution This problem calls for a determination of the number of atoms per cubic meter for chromium. In order to solve this problem, one must employ Equation 4.2,
N =
N A rCr ACr
The density of Cr (from the table inside of the front cover) is 7.19 g/cm3, while its atomic weight is 52.00 g/mol. Thus,
N=
(6.022 ´ 1023 atoms/mol)(7.19 g/cm3 ) 52.00 g/mol
= 8.33 ´ 1022 atoms/cm3 = 8.33 ´ 1028 atoms/m3
4.22 The concentration of Si in an FeSi alloy is 0.25 wt%. What is the concentration in kilograms of Si per cubic meter of alloy?
Solution In order to compute the concentration in kg/m3 of Si in a 0.25 wt% Si99.75 wt% Fe alloy we must employ Equation 4.9 as
CSi ¢¢ =
CSi
rSi
CSi ´ 103 CFe +
r Fe
From inside the front cover, densities for silicon and iron are 2.33 and 7.87 g/cm3, respectively; therefore
CSi ¢¢ =
0.25 0.25 2.33 g/cm 3
+
99.75 7.87 g/cm 3
= 19.6 kg/m3
´ 103
4.23 The concentration of phosphorus in silicon is 1.0 107 at%. What is the concentration in kilograms of phosphorus per cubic meter?
Solution Strategy for solving: Step 1: Convert the concentration of P from at% to wt% using Equation 4.7a Step 2: Compute the concentration of kilograms per cubic meter using Equation 4.9a
Step 1: From Equation 4.7a, the concentration of P in weight percent is determined as follows:
CP =
CP¢ AP ´ 100 CP¢ AP + CSi ¢ ASi
where
CFe ¢ = 1.0 107 at% CSi ¢ = 100.00 at% 1.0 107 at% = 99.9999999 at% AP = 30.97 g/mol (from inside front cover) ASi = 28.09 g/mol (from inside front cover) Now, solve for CP using the above equation
CP =
(1.0 ´ 107 at%)(30.97 g/mol) (1.0 ´ 107 at%)(30.97 g/mol) + (99.9999999 at%)(28.09 g.mol)
= 1.103 ´ 107 wt% Step 2 We now compute the number of kilograms per meter cubed (Equation 4.9a) with
Si = 2.33 g/cm3 (from inside front cover) P = 1.82 g/cm3 (from inside front cover) CSi = 100.00 wt% 1.103 ´ 107 wt% = 99.999999890 Therefore
æ ö ç C ÷ P ÷ ´ 103 CP¢¢ = ç ç CP CSi ÷ çr +r ÷ è P Si ø
´ 100
æ ö ç ÷ 1.103 ´ 107 wt% ç ÷ ´ 103 = ç 1.103 ´ 10 7 wt% 99.999999890 wt% ÷ ç ÷ + è ø 1.82 g/cm 3 2.33 g/cm 3
2.57 ´ 106 kg/m3
4.24 Determine the approximate density of a Ti6Al4V titanium (Ti) alloy that has a composition of 90 wt% Ti, 6 wt% Al, and 4 wt% V.
Solution In order to solve this problem, Equation 4.10a is modified to take the following form:
rave =
CTi
rTi
+
100 CAl
rAl
+
CV
rV
And, using the density values for Ti, Al, and Vâ€”i.e., 4.51 g/cm3, 2.71 g/cm3, and 6.10 g/cm3â€”(as taken from inside the front cover of the text), the density is computed as follows:
rave =
90 wt% 4.51 g/cm
3
+
100 6 wt% 2.71 g/cm
= 4.38 g/cm3
3
+
4 wt% 6.10 g/cm 3
4.25 Calculate the unit cell edge length for an 80 wt% Ag 20 wt% Pd alloy. All of the palladium is in solid solution, the crystal structure for this alloy is FCC, and the roomtemperature density of Pd is 12.02 g/cm3.
Solution In order to solve this problem it is necessary to employ Equation 3.8; in this expression density and atomic weight will be averages for the alloy—that is
rave =
nAave VC N A
Inasmuch as the unit cell is cubic, then VC = a3, then
rave =
nAave a3 N A
And solving this equation for the unit cell edge length, leads to
æ nAave ö a=ç ÷ è rave N A ø
1/3
Expressions for Aave and aveare found in Equations 4.11a and 4.10a, respectively, which, when incorporated into the above expression yields 1/3
é æ ö ù ê ç ÷ ú ê ç 100 ÷ ú ê nç C ÷ ú ê ç Ag + CPd ÷ ú ê çè A APd ÷ø ú Ag ú a= ê ö êæ ú êç ú ÷ êç 100 ÷N ú êç C ÷ Aú ê ç Ag + CPd ÷ ú ê çè rAg r Pd ÷ø ú ë û
Since the crystal structure is FCC, the value of n in the above expression is 4 atoms per unit cell. The atomic weights for Ag and Pd are 107.87 and 106.4 g/mol, respectively (Figure 2.8), whereas the densities for the Ag and Pd are 10.49 g/cm3 (inside front cover) and 12.02 g/cm3. Substitution of these, as well as the concentration values stipulated in the problem statement, into the above equation gives
é æ ö ê ç ÷ 100 ê (4 atoms/unit cell) ç ÷ ê 80 wt% 20 wt% ÷ ç ê çè 107.87 g/mol + 106.4 g/mol ÷ø a= ê êæ ö êç ÷ 100 êç ÷ 6.022 ´ 1023 atoms/mol ê ç 80 wt% 20 wt% ÷ + êç ÷ êë è 10.49 g/cm3 12.02 g/cm 3 ø
(
= 4.050 ´ 108 cm = 0.4050 nm
1/3
)
ù ú ú ú ú ú ú ú ú ú ú úû
4.26 Some hypothetical alloy is composed of 25 wt% of metal A and 75 wt% of metal B. If the densities of metals A and B are 6.17 and 8.00 g/cm3, respectively, and their respective atomic weights are 171.3 and 162.0 g/mol, determine whether the crystal structure for this alloy is simple cubic, facecentered cubic, or bodycentered cubic. Assume a unit cell edge length of 0.332 nm.
Solution In order to solve this problem it is necessary to employ Equation 3.8; in this expression density and atomic weight will be averages for the alloy—that is
rave =
nAave VC N A
Inasmuch as for each of the possible crystal structures, the unit cell is cubic, then VC = a3, or
rave =
nAave a3 N A
Now, in order to determine the crystal structure it is necessary to solve for n, the number of atoms per unit cell. For n =1, the crystal structure is simple cubic, whereas for n values of 2 and 4, the crystal structure will be either BCC or FCC, respectively. When we solve the above expression for n the result is as follows:
n=
rave a3N A Aave
Expressions for Aave and aveare found in Equations 4.11a and 4.10a, respectively, which, when incorporated into the above expression yields
æ ö ç 100 ÷ ç ÷ a3 N A ç CA C B ÷ çr +r ÷ è A Bø n= æ ö ç 100 ÷ ç ÷ ç CA CB ÷ ç A + A ÷ è A Bø Substitution of the concentration values (i.e., CA = 25 wt% and CB = 75 wt%) as well as values for the other parameters given in the problem statement, into the above equation gives
æ ö ç ÷ 100 ç ÷ (3.32 ´ 10 8 nm)3(6.022 ´ 1023 atoms/mol) ç 25 wt% + 75 wt% ÷ çè 6.17 g/cm 3 8.00 g/cm 3 ÷ø n= æ ö ç ÷ 100 ç ÷ ç 25 wt% + 75 wt% ÷ çè 171.3 g/mol 162.0 g/mol ÷ø = 1.00 atom/unit cell Therefore, on the basis of this value, the crystal structure is simple cubic.
4.27 For a solid solution consisting of two elements (designated as 1 and 2), sometimes it is desirable to determine the number of atoms per cubic centimeter of one element in a solid solution, N1, given the concentration of that element specified in weight percent, C1. This computation is possible using the following expression:
N1 =
C1A1
r1
N AC1 A + 1 (100  C1 )
(4.21)
r2
where NA is Avogadro’s number, ρ1 and ρ2 are the densities of the two elements, and A1 is the atomic weight of element 1. Derive Equation 4.21 using Equation 4.2 and expressions contained in Section 4.4.
Solution This problem asks that we derive Equation 4.21, using other equations given in the chapter. The concentration of component 1 in atom percent (C1¢ ) is just 100 c1¢ where c1¢ is the atom fraction of component 1. Furthermore, c1¢ is defined as c1¢ = N1/N where N1 and N are, respectively, the number of atoms of component 1 and total number of atoms per cubic centimeter. Thus, from the above discussion the following holds:
N1 =
C1¢ N 100
Substitution into this expression of the appropriate form of N from Equation 4.2 yields
N1 =
C1¢ N A rave 100 Aave
And, finally, substitution into this equation expressions for C1¢ (Equation 4.6a), ave (Equation 4.10a), Aave (Equation 4.11a), and realizing that C2 = (C1 – 100), and after some algebraic manipulation we obtain the desired expression:
N1 =
N AC1 C1 A1
r1
+
A1
r2
(100
 C1 )
4.28 Molybdenum (Mo) forms a substitutional solid solution with tungsten (W). Compute the number of molybdenum atoms per cubic centimeter for a molybdenumtungsten alloy that contains 16.4 wt% Mo and 83.6 wt% W. The densities of pure molybdenum and tungsten are 10.22 and 19.30 g/cm 3, respectively.
Solution This problem asks us to determine the number of molybdenum atoms per cubic centimeter for a 16.4 wt% Mo83.6 wt% W solid solution. To solve this problem, employment of Equation 4.21 is necessary, using the following values: C1 = CMo = 16.4 wt%
1 = Mo = 10.22 g/cm3 2 = W = 19.30 g/cm3 A1 = AMo = 95.94 g/mol Thus
N Mo =
N ACMo CMo AMo
rMo
=
+
AMo
rW
(100
 CMo )
(6.022 ´ 1023 atoms/mol) (16.4 wt%) (16.4 wt%)(95.94 g/mol) 10.22 g/cm
3
+
95.94 g/mol 19.3 g/cm3
= 1.73 1022 atoms/cm3
(100  16.4 wt%)
4.29 Niobium forms a substitutional solid solution with vanadium. Compute the number of niobium atoms per cubic centimeter for a niobiumvanadium alloy that contains 24 wt% Nb and 76 wt% V. The densities of pure niobium and vanadium are 8.57 and 6.10 g/cm3, respectively.
Solution This problem asks us to determine the number of niobium atoms per cubic centimeter for a 24 wt% Nb76 wt% V solid solution. To solve this problem, employment of Equation 4.21 is necessary, using the following values: C1 = CNb = 24 wt%
1 = Nb = 8.57 g/cm3 2 = V = 6.10 g/cm3 A1 = ANb = 92.91 g/mol Thus
N Nb =
CNb ANb
rNb
=
N ACNb A + Nb (100  CNb )
rV
(6.022 ´ 1023 atoms/mol) (24 wt%) (24 wt%)(92.91 g/mol) 8.57 g/cm
3
+
92.91 g/mol 6.10 g/cm3
= 1.02 1022 atoms/cm3
(100  24 wt%)
4.30 Consider an ironcarbon alloy that contains 0.2 wt% C, in which all the carbon atoms reside in tetrahedral interstitial sites. Compute the fraction of these sites that are occupied by carbon atoms.
Solution The following strategy will be used to solve this problem: Step 1: compute the number of Fe atoms per centimeter cubed using Equation 4.21 Step 2: compute the number of C atoms per centimeter cubed also using Equation 4.21 Step 3: compute the number of unit cells per centimeter cubed by dividing the number of Fe atoms per centimeter cubed (Step 1) by two since there are two Fe atoms per BCC unit cell Step 4: compute the number of total interstitial sites per centimeter cubed by multiplying the number of tetrahedral interstitial sites by the number of unit cells per cubic centimeter (from Step 3) Step 5: The fraction of tetrahedral sites occupied by carbon atoms is computed by dividing the number of carbon atoms per centimeter cubed (Step 3) by the total number of interstitial sites per cubic centimeter The solution to this problem involves using the following values: CC = 0.2 wt% CFe = 99.8 wt%
C = 2.25 g/cm3 Fe = 7.87 g/cm3 AC = 12.01 g/mol AFe = 55.85 g/mol Step 1: We compute the number of Fe atoms per cubic centimeter using Equation 4.21 as:
N Fe =
CFe AFe
rFe
=
N ACFe A + Fe (100  CFe )
rC
(6.022 ´ 1023 atoms/mol)(99.8 wt% Fe) (99.8 wt% Fe)(55.85 g/mol) (55.85 g/mol) + (100 wt%  99.8 wt%) 7.87 g/cm3 2.25 g/cm3
8.43 ´ 1022 Fe atoms/cm3 Step 2: We can compute the number of C atoms per cubic centimeter also using Equation 4.21 as follows:
NC =
N ACC CC AC AC + (100  CC )
rC
=
rFe
(6.022 ´ 1023 atoms/cm3 )(0.2 wt%) (0.2 wt%)(12.01 g/mol) 12.01 g/mol + (100 wt%  0.2 wt%) 2.25 g/cm3 7.87 g/cm3
= 7.85 ´ 1020 C atoms/cm3 Step 3: the number of unit cells per centimeter cubed is determined by dividing the number of Fe atoms per centimeter cubed (Step 1) by two since there are two Fe atoms per BCC unit cell—that is
no. unit cells/cm3 =
=
N Fe 2
8.43 ´ 1022 Fe atoms/cm3 = 4.22 ´ 1022 2
Step 4: We compute the number of total interstitial sites per centimeter cubed by multiplying the number of tetrahedral interstitial sites per unit cell by the number of unit cells per cubic centimeter (from Step 3). From Figure 4.3b, there are 4 tetrahedral sites located on the front face plane of the unit cell—one site for each of the unit cell edges in this plane. Inasmuch as there are 6 faces on this unit cell there are 6 4 = 24 interstitial sites for this unit cell. However, each of these sites is shared by 2 unit cells, which means that only 12 sites belong to each unit cell. Therefore the number of tetrahedral sites per centimeter cubed corresponds to 12 times the number of unit cells per cubic centimeter (ns)—that is
ns = (12 sites/unit cell)(4.22 ´ 1022 unit cells/cm3 )
= 5.06 ´ 1023 sites/cm3 Step 5: The fraction of tetrahedral sites occupied by carbon atoms is computed by dividing the number of carbon atoms per centimeter cubed (Step 3) by the total number of interstitial sites per cubic centimeter, that is
fraction sites occupied =
NC ns
=
7.85 ´ 1020 C atoms/cm3 5.06 ´ 1023 sites/cm3
= 1.55 ´ 103
4.31 For a BCC ironcarbon alloy that contains 0.1 wt% C, calculate the fraction of unit cells that contain carbon atoms.
Solution It is first necessary to compute the number of carbon atoms per cubic centimeter of alloy using Equation 4.21. For this problem A1 = AC = 12.011 g/mol (from inside the front cover) C1 = CC = 0.1 wt%
1 = C = 2.25 g/cm3 (from inside front cover) 2 = Fe = 7.87 g/cm3 (from inside front cover) Now using from Equation 4.21
NC =
N ACC CC AC AC + (100  CC )
rC
=
r Fe
(6.022 ´ 1023atoms/mol)(0.1 wt%) (0.1 wt%)(12.011 g/mol) (12.011 g/mol) + (100  0.1 wt%) 2.25 g/cm3 7.87 g/cm3 = 3.94 1020 C atoms/cm3
We now perform the same calculation for iron atoms, where A1 = AFe = 55.85 g/mol (from inside the front cover) C1 = CFe = 100% 0.1 wt% = 99.9 wt%
1 = Fe = 7.87 g/cm3 (from inside front cover) 2 = C = 2.25 g/cm3 (from inside front cover) Therefore,
=
(6.022 ´ 1023atoms/mol)(99.9 wt%) (99.9 wt%)(55.85 g/mol) (55.85 g/mol) + (100  99.9 wt%) 7.87 g/cm3 2.25 g/cm3 = 8.46 1022 Fe atoms/cm3
From Section 3.4 there are two Fe atoms associated with each unit cell; hence, the number of unit cells in a centimeter cubed, ni, is equal to
ni =
=
No. Fe atoms/cm3 No. atoms/unit cell
8.46 ´ 10 22 atoms/cm3 = 4.23 ´ 1022 unit cells/cm3 2 atoms/unit cell
Now, the fraction of unit cells that contain carbon atoms, nf , is just the number of carbon atoms per centimeter cubed (3.94 1020) divided by the number of unit cells per centimeter cubed (4.23 1022), or
nf =
3.94 ´ 1020 C atoms/cm3 4.23 ´ 1022 unit cells/cm3
= 9.31 ´ 103 atoms/unit cell The reciprocal of nf is the number of unit cells per atom—viz.
1 1 = n f 9.31 ´ 10 3 atoms/unit cell
=107.5 unit cells/atom That is, there is one carbon atom per 107.5 unit cells.
4.32 For Si to which has had added 1.0 105 at% of aluminum (Al), calculate the number of Al atoms per cubic meter.
Solution To make this computation we need to use Equation 4.21. However, because the concentration of Al is given in atom percent, it is necessary to convert 1.0 105 at% to weight percent using Equation 4.7a. For this computation C1 = CAl = concentration of Al in wt%
C1¢ = CAl ¢ atom percent of Al = 1.0 105 at%
C2¢ = CSi ¢ atom percent of Si = 100 at% 1.0 105 at% = 99.99999 at% A1 = AAl = atomic weight of Al = 26.98 g/mol (from inside front cover) A2 = ASi = atomic weight of Si = 28.09 g/mol (from inside front cover) Now using Equation 4.7a we compute the value of C1 (or CAl) as follows:
C1 =
=
C1¢A1 ´ 100 C1¢A1 + C2¢ A2
(1.0 ´ 105 wt%)(26.98 g/mol) (1.0 ´ 105 wt%)(26.98 g/mol) + (99.99999 wt%)(28.09 g/mol) 9.60 106 wt%
Now employment of Equation 4.21 with N1= number of Al atoms per meter cubed C1 = concentration of Al in weight percent = 9.60 106 wt% A1 = atomic weight of Al = 26.98 g/mol (inside front cover)
1 = density of Al = 2.71 g/cm3 (inside front cover)
2 = density of silicon = 2.33 g/cm3 (inside front cover)
leads to
N1 =
N AC1 C1 A1 A1 + (100  C1 )
r1
r2
´ 100
=
(6.022 ´ 1023 atoms/mol)(9.60 ´ 106 wt%) (9.60 ´ 106 wt%)(26.98 g/mol) 2.71 g/cm
3
+
(26.98 g/mol) 2.33 g/cm3
(100  9.60 ´ 106 wt%)
= 4.99 1015 Al atoms/cm3
4.33 Sometimes it is desirable to determine the weight percent of one element, C1, that will produce a specified concentration in terms of the number of atoms per cubic centimeter, N1, for an alloy composed of two types of atoms. This computation is possible using the following expression:
C1 =
100 N A r2 r2 1+ N1A1 r1
(4.22)
where NA is Avogadro’s number, ρ1 and ρ2 are the densities of the two elements, and A1 is the atomic weight of element 1. Derive Equation 4.22 using Equation 4.2 and expressions contained in Section 4.4.
Solution This problem asks that we derive Equation 4.22, using other equations given in the chapter. The number of atoms of component 1 per cubic centimeter is just equal to the atom fraction of component 1 (c1¢ ) times the total number of atoms per cubic centimeter in the alloy (N). Thus, using the equivalent of Equation 4.2 for N, we may write
N1 = c1¢ N =
c¢N A rave Aave
Realizing that
c1¢ =
C1¢ 100
and
C2¢ = 100  C1¢ and substitution of the expressions for and A , Equations 4.10b and 4.11b, respectively, leads to ave ave
N1 =
c1¢ N A rave Aave
æ ö ç C1¢ A1 + C2¢ A2 ÷ (c1¢ N A ) ç C ¢A C ¢ A ÷ ç 1 1+ 2 2÷ r2 ø è r1 = C ¢A1 + C2¢ A2 100
=
N AC1¢ r1 r2 C1¢ r2 A1 + (100  C1¢ ) r1 A2
And, solving for C1¢ leads to
C1¢ =
100 N1 r1 A2 N A r1 r2  N1 r2 A1 + N1 r1 A2
Substitution of this expression for C1¢ into Equation 4.7a, which may be written in the following form
æ ö 100 N1 r1 A2 ç ÷ A1 è N A r1 r2  N1 r2 A1 + N1 r1 A2 ø C1 = ´ 100 é æ ö æ öù 100 N1 r1 A2 100 N1 r1 A2 ç ÷ A1 + ê100  ç ÷ ú A2 êë è N A r1 r2  N1 r2 A1 + N1 r1 A2 ø è N A r1 r2  N1 r2 A1 + N1 r1 A2 ø úû
which simplifies to
C1 =
the desired expression.
100 1+
N A r2 r2 N1 A1 r1
4.34 Gold (Au) forms a substitutional solid solution with silver (Ag). Compute the weight percent of gold that must be added to silver to yield an alloy that contains 5.5 × 10 21 Au atoms per cubic centimeter. The densities of pure Au and Ag are 19.32 and 10.49 g/cm 3, respectively.
Solution To solve this problem, employment of Equation 4.22 is necessary, using the following values: N1 = NAu = 5.5 1021 atoms/cm3
1 = Au = 19.32 g/cm3 2 = Ag = 10.49 g/cm3 A1 = AAu = 196.97 g/mol (found inside front cover) A2 = AAg = 107.87 g/mol (found inside from cover)
Thus
100
CAu = 1+
N A rAg N Au AAu

rAg rAu
100
= 1+
æ 10.49 g/cm 3 ö ç ÷ (5.5 ´ 1021 atoms/cm3 )(196.97 g/mol) è 19.32 g/cm3 ø
(6.022 ´
1023 atoms/mol
)(10.49 g/cm3 )
= 15.9 wt%
4.35 Germanium (Ge) forms a substitutional solid solution with silicon (Si). Compute the weight percent of germanium that must be added to silicon to yield an alloy that contains 2.43 × 10 21 Ge atoms per cubic centimeter. The densities of pure Ge and Si are 5.32 and 2.33 g/cm 3, respectively.
Solution To solve this problem, employment of Equation 4.22 is necessary, using the following values: N1 = NGe = 2.43 1021 atoms/cm3
1 = Ge = 5.32 g/cm3 2 = Si = 2.33 g/cm3 A1 = AGe = 72.64 g/mol (found inside front cover) A2 = ASi = 28.09 g/mol (found inside front cover)
Thus
CGe =
100 N A rSi r 1+  Si N Ge AGe rGe
100
= 1+
æ 2.33 g/cm 3 ö ç ÷ (2.43 ´ 1021 atoms/cm3 ) (72.64 g/mol) è 5.32 g/cm3 ø
(6.022 ´
1023 atoms/mol
)(2.33 g/cm3 )
= 11.7 wt%
4.36 Electronic devices found in integrated circuits are composed of very high purity silicon to which has been added small and very controlled concentrations of elements found in Groups IIIA and VA of the periodic table. For Si to which has had added 6.5 1021 atoms per cubic meter of phosphorus, compute (a) the weight percent and (b) the atom percent of P present.
Solution (a) This part of the problem is solved using Equation 4.22, in which C1 = concentration of P in wt% N1 = number of P atoms per cubic centimeter = (6.5 1021 atoms/m3)(1 m3/106 cm3) = 6.5 1015 atoms/cm3 A1 = atomic weight of P = 30.97 g/mol (inside front cover)
1 = density of P = 1.82 g/cm3 (inside front cover) 2 = density of silicon = 2.33 g/cm3 (inside front cover) And, from Equation 4.22
C1 =
100 N A r2 r2 1+ N1A1 r1
100
= 1+
(6.022 ´ 10
23
atoms/mol)(2.33 g/cm3 )
(6.5 ´ 1015 atoms/cm3 )(30.97 g/mol)

2.33 g/cm3 1.82 g/cm3
= 1.43 105 wt% (b) To convert from weight percent to atom percent we use Equation 4.6a where
C1¢ = atom percent of P C1 = weight percent of P = 1.43 105 wt% C2 = weight percent of Si = 100 wt% 1.43 105 wt% = 99.9999857 A1 = atomic weight of P = 30.97 g/mol A2 = atomic weight of Si = 28.09 g/mol And from Equation 4.6a we obtain the following:
C1¢ =
=
C1A2 ´ 100 C1A2 + C2 A1
(1.43 ´ 105 wt%)(28.09 g/mol) (1.43 ´ 105 wt%)(28.09 g/mol) + (99.9999857 wt%)(30.97 g/mol) = 1.30 105 at%
´ 100
4.37 Iron and vanadium both have the BCC crystal structure, and V forms a substitutional solid solution for concentrations up to approximately 20 wt% V at room temperature. Compute the unit cell edge length for a 90 wt% Feâ€“10 wt% V alloy.
Solution This problems asks that we compute the unit cell edge length for a 90 wt% Fe10 wt% V alloy. First of all, the atomic radii for Fe and V (using the table inside the front cover) are 0.124 and 0.132 nm, respectively. Also, using Equation 3.8 it is possible to compute the unit cell volume, and inasmuch as the unit cell is cubic, the unit cell edge length is just the cube root of the volume. However, it is first necessary to calculate the density and average atomic weight of this alloy using Equations 4.10a and 4.11a. Inasmuch as the densities of iron and vanadium are 7.87g/cm3 and 6.10 g/cm3, respectively, (as taken from inside the front cover), the average density is just
rave =
100 CV CFe +
rV
=
r Fe
100 10 wt% 6.10 g/cm
3
+
90 wt% 7.87 g/cm 3
= 7.65 g/cm3 And for the average atomic weight
Aave =
=
100 CV CFe + AV AFe
100 10 wt% 90 wt% + 50.94 g/mol 55.85 g/mol
= 55.32 g/mol Now, VC is determined from Equation 3.8 as (taking the number of atoms per unit cell, n = 2, since the crystal structure of the alloy is BCC)
VC =
=
nAave rave N A
(2 atoms/unit cell)(55.32 g/mol)
(7.65 g/cm3)(6.022 ´
1023 atoms/mol)
= 2.40 1023 cm3/unit cell And, finally, because the unit cell is of cubic symmetry
a = (VC )1/3 = (2.40 ´ 10 23 cm3 /unit cell)1/3 = 2.89 108 cm = 0.289 nm
Dislocationsâ€”Linear Defects 4.38 Cite the relative Burgers vectorâ€“dislocation line orientations for edge, screw, and mixed dislocations. Answer The Burgers vector and dislocation line are perpendicular for edge dislocations, parallel for screw dislocations, and neither perpendicular nor parallel for mixed dislocations
Interfacial Defects 4.39 For an FCC single crystal, would you expect the surface energy for a (100) plane to be greater or less than that for a (111) plane? Why? (Note: You may want to consult the solution to Problem 3.60 at the end of Chapter 3.) Answer The surface energy for a crystallographic plane will depend on its packing density [i.e., the planar density (Section 3.11)]â€”that is, the higher the packing density, the greater the number of nearestneighbor atoms, and the more atomic bonds in that plane that are satisfied, and, consequently, the lower the surface energy. From the 1 1 solution to Problem 3.60, planar densities for FCC (100) and (111) planes are and , respectivelyâ€”that 2R 2 3 4R 2 0.25 0.29 is and (where R is the atomic radius). Thus, since the planar density for (111) is greater, it will have the 2 R R2 lower surface energy.
4.40 For a BCC single crystal, would you expect the surface energy for a (100) plane to be greater or less than that for a (110) plane? Why? (Note: You may want to consult the solution to Problem 3.61 at the end of Chapter 3.) Answer The surface energy for a crystallographic plane will depend on its packing density [i.e., the planar density (Section 3.11)]â€”that is, the higher the packing density, the greater the number of nearestneighbor atoms, and the more atomic bonds in that plane that are satisfied, and, consequently, the lower the surface energy. From the 3 3 solution to Problem 3.61, the planar densities for BCC (100) and (110) are and , respectivelyâ€”that 2 2 8R 2 16R 0.19 0.27 is and . Thus, since the planar density for (110) is greater, it will have the lower surface energy. 2 R R2
4.41 For a single crystal of some hypothetical metal that has the simple cubic crystal structure (Figure 3.3), would you expect the surface energy for a (100) plane to be greater, equal to, or less than a (110) plane. Why? Answer The surface energy for a crystallographic plane will depend on its packing density [i.e., the planar density (Section 3.11)]â€”that is, the higher the packing density, the greater the number of nearestneighbor atoms, and the more atomic bonds in that plane that are satisfied, and, consequently, the lower the surface energy. It becomes necessary to determine the packing densities of the (100) and (110) planes for the simple cubic crystal structure. Below is shown a (100) plane for simple cubic.
For this plane there is one atom at each of the four corners, which is shared with four adjacent unit cells. Thus there is the equivalence of one atom associated with this (100) plane. The planar section is a square, where in the side 2
lengths are equal to the unit cell edge length, 2R. Thus the area of this square is 4R , which yields a planar density of number of atoms centered on the (100) plane PD100 = area of (100) plane
=
1 atom 4R
2
=
0.25 R2
We now repeat this procedure for a (110) plane, which is shown below.
Because each of these atoms is shared with four other unit cells, there is the equivalence of 1 atom associated with the plane. This planar section is a rectangle with dimensions of 2R Â´ 2R 2 (Note: 2 2 = 2.83 ). Thus the area of this rectangle is 4R2 2 = 5.66R2 . The planar density for the (110) plane is, therefore,
PD110 =
1 atom 5.66R
2
=
0.18 R2
Thus, because the planar density for (100) is greater, it will have the lower surface energy.
4.42 (a) For a given material, would you expect the surface energy to be greater than, the same as, or less than the grain boundary energy? Why? (b) The grain boundary energy of a smallangle grain boundary is less than for a highangle one. Why is this so? Answer (a) The surface energy will be greater than the grain boundary energy. For grain boundaries, some atoms on one side of a boundary will bond to atoms on the other side; such is not the case for surface atoms. Therefore, there will be fewer unsatisfied bonds along a grain boundary. (b) The smallangle grain boundary energy is lower than for a highangle one because more atoms bond across the boundary for the smallangle, and, thus, there are fewer unsatisfied bonds.
4.43 (a) Briefly describe a twin and a twin boundary. (b) Cite the difference between mechanical and annealing twins. Answer (a) A twin boundary is an interface such that atoms on one side are located at mirror image positions of those atoms situated on the other boundary side. The region on one side of this boundary is called a twin. (b) Mechanical twins are produced as a result of mechanical deformation and generally occur in BCC and HCP metals. Annealing twins form during annealing heat treatments, most often in FCC metals.
4.44 For each of the following stacking sequences found in FCC metals, cite the type of planar defect that exists: (a) . . . A B C A B C B A C B A . . . (b) . . . A B C A B C B C A B C . . . Copy the stacking sequences, and indicate the position(s) of planar defect(s) with a vertical dashed line. Answer (a) The interfacial defect that exists for this stacking sequence is a twin boundary, which occurs at the indicated position.
The stacking sequence on one side of this position is mirrored on the other side.
(b) The interfacial defect that exists within this FCC stacking sequence is a stacking fault, which occurs between the two lines.
Within this region, the stacking sequence is HCP.
Grain Size Determination 4.45 (a) Using the intercept method determine the mean intercept length, in millimeters, of the specimen whose microstructure is shown in Figure 4.15b; use at least seven straightline segments. (b) Estimate the ASTM grain size number for this material. Solution (a) Below is shown the photomicrograph of Figure 4.15b, on which seven straight line segments, each of which is 60 mm long has been constructed; these lines are labeled ―1‖ through ―7‖.
Since the length of each line is 60 mm and there are 7 lines, the total line length (LT in Equation 4.16) is 420 mm. Tabulated below is the number of grainboundary intersections for each line: Line Number
No. Grains Intersected
1
11
2
10
3
9
4
8.5
5
7
6
10
7
8
Total
63.5
Because LT = 420 mm, P = 63.5 grainboundary intersections, and the magnification M = 100ď‚´, the mean intercept length
is computed using Equation 4.16 as follows:
=
LT 420 mm = PM (63.5 intersections)(100Â´)
= 0.066 mm
(b) The ASTM grain size number G is computed by substitution of this value for follows:
G = 6.6457log  3.298
= (6.6457)[log(0.066 mm)] 3.298 = 4.55
into Equation 4.19a as
4.46 (a) Employing the intercept technique, determine the mean intercept length for the steel specimen whose microstructure is shown in Figure 9.25a; use at least seven straightline segments. (b) Estimate the ASTM grain size number for this material. Solution (a) Below is shown the photomicrograph of Figure 9.25a, on which seven straight line segments, each of which is 60 mm long has been constructed; these lines are labeled ―1‖ through ―7‖.
Since the length of each line is 60 mm and there are 7 lines, the total line length (LT in Equation 4.16) is 420 mm. Tabulated below is the number of grainboundary intersections for each line: Line Number
No. Grains Intersected
1
7
2
7
3
7
4
8
5
10
6
6
7
8
Total
53
Because LT = 420 mm, P = 56 grainboundary intersections, and the magnification M = 90ď‚´, the mean intercept length
is computed using Equation 4.16 as follows:
=
LT 420 mm = PM (53 intersections)(90Â´)
= 0.088 mm
(b) The ASTM grain size number G is computed by substitution of this value for follows:
G = 6.6457log  3.298
= (6.6457)[log(0.088 mm)] 3.298 = 3.72
into Equation 4.19a as
4.47 For an ASTM grain size of 6, approximately how many grains would there be per square inch under each of the following conditions? (a) At a magnification of 100 (b) Without any magnification? Solution (a) This part of problem asks that we compute the number of grains per square inch for an ASTM grain size of 6 at a magnification of 100. All we need do is solve for the parameter n in Equation 4.17, inasmuch as G = 6. Thus
n = 2G 1 = 261 = 32 grains/in.2
(b) Now it is necessary to compute the value of n for no magnification. In order to solve this problem it is necessary to use Equation 4.18: 2
æ Mö nM ç = 2G 1 è 100 ÷ø
where nM = the number of grains per square inch at magnification M, and G is the ASTM grain size number. Without any magnification, M in the above equation is 1, and therefore, 2
æ 1 ö n1 ç = 261 = 32 è 100 ÷ø And, solving for n1, n1 = 320,000 grains/in.2.
4.48 Determine the ASTM grain size number if 30 grains per square inch are measured at a magnification of 250. Solution In order to solve this problem we make use of Equation 4.18: 2
æ Mö nM ç = 2G 1 è 100 ÷ø
where nM = the number of grains per square inch at magnification M, and G is the ASTM grain size number. Solving the above equation for G, and realizing that nM = 30, while M = 250. Some algebraic manipulation of Equation 4.18 is necessary. Taking logarithms of both sides of this equation leads to
é æ M ö2ù G1 log ênM ç ÷ø ú = log 2 è 100 êë úû
( )
Or
æ Mö log nM + 2 log ç = (G 1)log 2 è 100 ÷ø And solving this equation for G
æ M ö lognM + 2 log ç è 100 ÷ø = G 1 log 2 or
æ M ö log nM + 2 log ç è 100 ÷ø G= +1 log 2 From the problem statement: nM =30 M = 250 And, therefore
æ 250 ö log 30 + 2 log ç è 100 ÷ø G= + 1 = 8.6 log 2
4.49 Determine the ASTM grain size number if 25 grains per square inch are measured at a magnification of 75. Solution In order to solve this problem we make use of Equation 4.18—viz. 2
æ Mö nM ç = 2G 1 è 100 ÷ø
where nM = the number of grains per square inch at magnification M, and G is the ASTM grain size number. By algebraic manipulation of Equation 4.18 (as outlined in Problem 4.48) we make G the dependent variable, which leads to the following expression:
æ M ö log nM + 2 log ç è 100 ÷ø G= +1 log 2 For nM = 25 and M = 75, the value of G is
æ 75 ö log 25 + 2 log ç è 100 ÷ø G= + 1 = 4.8 log 2
4.50 The following is a schematic micrograph that represents the microstructure of some hypothetical metal.
Determine the following: (a) Mean intercept length (b) ASTM grain size number, G Solution (a) Below is shown this photomicrograph on which six straight line segments, each of which is 50 mm long has been constructed; these lines are labeled ―1‖ through ―6‖.
Since the length of each line is 50 mm and there are 6 lines, the total line length (LT in Equation 4.16) is 300 mm. Tabulated below is the number of grainboundary intersections for each line:
Line Number
No. Grains Intersected
1
7
2
8
3
8
4
8
5
8
6
8
Total
47
Because LT = 300 mm, P = 47 grainboundary intersections, and the magnification M = 200ď‚´, the mean intercept length
is computed using Equation 4.16 as follows:
=
LT 300 mm = PM (47 intersections)(200Â´)
= 0.032 mm
(b) The ASTM grain size number G is computed by substitution of this value for follows:
G = 6.6457log  3.298
= (6.6457)[log(0.032 mm)] 3.298 = 6.64
into Equation 4.19a as
4.51 The following is a schematic micrograph that represents the microstructure of some hypothetical metal.
Determine the following: (a) Mean intercept length (b) ASTM grain size number, G Solution (a) Below is shown this photomicrograph on which six straight line segments, each of which is 50 mm long has been constructed; these lines are labeled ―1‖ through ―6‖.
Since the length of each line is 50 mm and there are 6 lines, the total line length (LT in Equation 4.16) is 300 mm. Tabulated below is the number of grainboundary intersections for each line:
Line Number
No. Grains Intersected
1
8
2
9
3
10
4
8
5
9
6
8
Total
52
Because LT = 300 mm, P = 52 grainboundary intersections, and the magnification M = 150ď‚´, the mean intercept length
is computed using Equation 4.16 as follows:
=
LT 300 mm = PM (52 intersections)(150Â´)
= 0.038 mm
(b) The ASTM grain size number G is computed by substitution of this value for follows:
G = 6.6457log  3.298
= (6.6457)[log(0.038 mm)] 3.298 6.14
into Equation 4.19a as
DESIGN PROBLEMS Specification of Composition 4.D1 Aluminum–lithium (AlLi) alloys have been developed by the aircraft industry to reduce the weight and improve the performance of its aircraft. A commercial aircraft skin material having a density of 2.47 g/cm 3 is desired. Compute the concentration of Li (in wt%) that is required. Solution Solution of this problem requires the use of Equation 4.10a, which takes the form
rave =
100 100 = CLi CAl CLi 100  CLi + +
rLi
rAl
rLi
rAl
inasmuch as CLi + CAl = 100. According to the table inside the front cover, the respective densities of Li and Al are 0.534 and 2.71 g/cm3. Upon algebraic manipulation of the above equation and solving for CLi leads to
CLi =
100 rLi ( rAl  rave ) rave ( rAl  r Li )
Incorporation of values for ave, Al, and Li yields the following value for CLi:
CLi =
(100) (0.534 g/cm3 )(2.71 g/cm3  2.47 g/cm3 )
(2.47 g/cm3)(2.71 g/cm3  0.534 g/cm3) = 2.38 wt%
4.D2 Copper (Cu) and platinum (Pt) both have the FCC crystal structure, and Cu forms a substitutional solid solution for concentrations up to approximately 6 wt% Cu at room temperature. Determine the concentration in weight percent of Cu that must be added to Pt to yield a unit cell edge length of 0.390 nm. Solution To begin, it is necessary to employ Equation 3.8, and solve for the unit cell volume, VC, as
VC =
nAave rave N A
where Aave and ave are the atomic weight and density, respectively, of the PtCu alloy. Inasmuch as both of these materials have the FCC crystal structure, which has cubic symmetry, VC is just the cube of the unit cell length, a. That is
VC = a3 = (0.390 nm)3
= (3.90 ´ 108 cm)3 = 5.932 ´ 1023 cm3 It is now necessary to construct expressions for Aave and ave in terms of the concentration of copper, CCu, using Equations 4.11a and 4.10a. For Aave we have
Aave =
=
CCu ACu
100 (100  CCu ) + APt
100 CCu (100  CCu ) + 63.55 g/mol 195.08 g/mol
since the atomic weights for Cu and Pt are, respectively, 63.55 and 195.08 g/mol (as noted inside the front cover). Now, the expression for is as follows: ave
rave =
100 CCu
rCu
+
(100  CCu ) r Pt
=
100 CCu (100  CCu ) + 3 8.94 g/cm 21.45 g/cm 3
given the densities of 8.94 and 21.45 g/cm3 for the respective metals. Within the FCC unit cell there are 4 equivalent atoms, and thus, the value of n in Equation 3.8 is 4; hence, the expression for VC may be written in terms of the concentration of Cu in weight percent as follows:
VC = 5.932 ´ 1023 cm3
=
nAave rave N A
é ù ê ú 100 ú (4 atoms/unit cell) ê CCu (100  CCu ) ú ê ê 63.55 g/mol + 195.08 g/mol ú ë û = é ù ê ú 100 ê ú (6.022 ´ 1023 atoms/mol) ê CCu (100  CCu ) ú + ê ú êë 8.94 g/cm 3 21.45 g/cm 3 úû
And solving this expression for CCu leads to CCu = 2.825 wt%.
FUNDAMENTALS OF ENGINEERING QUESTIONS AND PROBLEMS 4.1FE Calculate the number of vacancies per cubic meter at 1000°C for a metal that has an energy for vacancy formation of 1.22 eV/atom, a density of 6.25 g/cm 3, and an atomic weight of 37.4 g/mol. (A) 1.49 1018 m3 (B) 7.18 1022 m3 (C) 1.49 1024 m3 (D) 2.57 1024 m3 Solution Determination of the number of vacancies per cubic meter at 1000C (1273 K) requires the utilization of Equations 4.1 and 4.2 as follows:
æ Q ö N r Nv = N exp ç  v ÷ = A exp è kT ø A
æ Qv ö çè  ÷ø kT
Incorporation into this expression values for Qv, and A provided in the problem statement yields the following for Nv:
Nv =
é ù (6.022 ´ 1023atoms/mol)(6.25 g/cm3 ) 1.22 eV/atom exp ê ú 5 37.4 g/mol êë (8.62 ´ 10 eV/atomK)(1273 K) úû = 1.49 1018 cm3 = 1.49 1024 m3
which is answer C.
4.2FE What is the composition, in atom percent, of an alloy that consists of 4.5 wt% Pb and 95.5 wt% Sn? The atomic weights for Pb and Sn are 207.19 g/mol and 118.71 g/mol, respectively. (A) 2.6 at% Pb and 97.4 at% Sn (B) 7.6 at% Pb and 92.4 at% Sn (C) 97.4 at% Pb and 2.6 at% Sn (D) 92.4 at% Pb and 7.6 at% Sn Solution We are asked to compute the composition of an alloy in atom percent. Employment of Equation 4.6a leads to
CPb ¢ =
=
CPb ASn ´100 CPb ASn + CSn APb
(4.5)(118.71 g/mol) ´ 100 (4.5)(118.71 g/mol) + (95.5)(207.19 g/mol)
= 2.6 at%
CSn ¢ =
=
CSn APb ´ 100 CSn APb + CPb ASn
(95.5)(207.19 g/mol) ´100 (95.5)(207.19 g/mol) + (4.5)(118.71 g/mol) = 97.4 at%
which is answer A (2.6 at% Pb and 97.4 at% Sn).
4.3FE What is the composition, in weight percent, of an alloy that consists of 94.1 at% Ag and 5.9 at% Cu? The atomic weights for Ag and Cu are 107.87 g/mol and 63.55 g/mol, respectively. (A) 9.6 wt% Ag and 90.4 wt% Cu (B) 3.6 wt% Ag and 96.4 wt% Cu (C) 90.4 wt% Ag and 9.6 wt% Cu (D) 96.4 wt% Ag and 3.6 wt% Cu Solution To compute composition, in weight percent, of a 94.1 at% Ag5.9 at% Cu alloy, we employ Equation 4.7 as follows:
CAg =
=
CAg ¢ AAg ´ 100 CAg ¢ AAg + CCu ¢ ACu
(94.1)(107.87 g/mol) ´ 100 (94.1)(107.87 g/mol) + (5.9)(63.55 g/mol) = 96.4 wt%
CCu =
=
CCu ¢ ACu ´ 100 CAg ¢ AAg + CCu ¢ ACu
(5.9)(63.55 g/mol) ´ 100 (94.1)(107.87 g/mol) + (5.9)(63.55 g/mol) = 3.6 wt%
which is answer D (96.4 wt% Ag and 3.6 wt% Cu).
Product details Language: English ISBN10: 1118324579 ISBN13: 9781118324578 9781118324578 Link full dow...
Published on Mar 13, 2018
Product details Language: English ISBN10: 1118324579 ISBN13: 9781118324578 9781118324578 Link full dow...